leaching and water uptake - spie.org resist leaching and water uptake 59 figure 3.5 leaching test...
Post on 14-Mar-2020
Embed Size (px)
Resist Leaching and Water Uptake
One unique aspect of 193i lithography is the use of water situated between the
final lens element and the resist. The resist stack (with or without topcoat) on the
wafer is dynamically exposed through this water with the step-and-scan process.
The photoacid generator (PAG), quencher, and other small molecular
components of the resist may leach into this water. These leached components
contaminate the water and may degrade resist performance. This contaminated
water can additionally contaminate the lens and wafer stage of the scanner. To
master these leaching problems, we must understand the dynamics of resist
leaching, transportation of leached contaminates in the immersion water, and the
impact of these contaminants on the lens during exposure.
Additionally, water can penetrate the topcoat and diffuse into the resist film.
This penetration and diffusion of water can cause the topcoat or the resist to swell,
which will affect their lithographic performance. This chapter specifically
addresses the following issues: (1) leaching test methods, (2) leaching dynamics,
(3) leaching with 193-nm exposure, (4) pre-rinse to partially remove leached
contaminants, (5) lens contamination caused by resist leaching, and (6) water
uptake in resist film.
3.1 Leaching Test Methods
A general approach to evaluating the leaching characteristics of a resist involves
several steps. First, a puddle of DI water is formed on the surface of the resist
stack. After a specific period of time, the water in the puddle is sent for analysis.
This leaching test measures the amount of resist components that are leached into
the water over time. Various methods of immersing the resist film and extracting
the water sample have been developed and reported, 1 however, the results have
been inconsistent with variability as high as 2–3x. So far, no standard test method
or specifications for leaching have been accepted by the entire 193i community.
However, these are worthwhile goals and more reliable methods continue to be
54 Chapter 3
3.1.1 Water extraction
Figure 3.1 shows a simple water extraction test method. 3 Although this method is
not recommended, it gives a basic example of water extraction. A beaker with a
wide opening (crystallizing dish) holds a specific volume of DI water (Fig.
3.1(a)). A silicon wafer coated with resist or resist stack is placed face down
covering the beaker mouth (Fig. 3.1(b)). The beaker and the wafer are flipped
over and the water covers the resist surface (Fig. 3.1(c)). The immersion area or
resist leaching area is equal to the size of the beaker opening. After a specific
amount of time, the beaker is flipped back to its normal position and the water is
collected for analysis (Fig. 3.1(d)). To investigate the time dependence of
leaching, a series of experiments can be conducted as a function of retention time.
Two recommended methods for this investigation are the Water EXtraction
and Analysis (WEXA) technique described by IBM 4 and the Dynamic Leaching
Procedure (DLP) developed at IMEC. 5 Figure 3.2(a) shows a diagram of the
bottom view of a Teflon lid in the WEXA design. In the test, the lid covers the
resist surface and the evacuation hole is connected to a vacuum pump. The gap
between the wafer and the lid is filled with water. Water flows along the
rectangular channel, reaching the outlet. The contact time with water can be
varied by adjusting the flow rate and the size of the channel. The water flowing
out of the outlet hole is collected for analysis.
Figure 3.2(b) is a diagram of how the DLP works. A resist-coated wafer is
loaded onto the wafer stage. A showerhead dispenses a specific volume of water
across the resist surface. Then, the water in the showerhead is collected for
analysis. The retention time of water contact can be varied by adjusting the speed.
Figure 3.1 Simple method of extracting a water sample from the resist surface using a
Resist Leaching and Water Uptake 55
Figure 3.2 Diagrams of (a) WEXA cover design (bottom view) and (b) how DPL works.
3.1.2 Water sample analysis
Water samples can be analyzed for resist components using various chemical
analytical methods that have different sensitivities toward certain components.
The best analytical method must be chosen for each compound. For example,
sulfonates of PAG can be detected separately by liquid chromatography mass
spectroscopy (LC-MS) with a detection limit of 0.2ng/mL or ppb. The dynamic
leaching rate (ng/cm 2 s) can be determined from quantitative measurements,
contact area, and immersion time. SEMATECH experiments suggest that the
PAGs are most likely to leach from the film and also impose the greatest danger
to the lens. 6 Experimental results from resist vendors also support this suggestion.
56 Chapter 3
3.2 Leaching Dynamics
3.2.1 Leaching dynamics described by a single-exponential model
The rate of leaching has been shown to be nonlinear. The resist components
(primarily PAGs) leach faster at the beginning of contact with water. Radioactive
labeling studies and early kinetics studies with limited time resolution have
shown that leaching reaches a limiting value within a few seconds after water
contact. 6 The concentration C of PAG in water versus the water contact time t
can be approximately described by an exponential relation:
C = C∞∙(1–e -βt
where C∞ is the saturated PAG concentration and β is the time constant. 7 The
leaching rate dC/dt changes with time. At initial time t = 0, the leaching rate has
the maximum value—dC/dt |t=0 = C∞∙β, which is called the dynamic leaching rate.
Both C∞ and C∞∙β can be obtained from the C–t curve (Fig. 3.3).
3.2.2 Leaching dynamics described by double-exponential model
Detailed measurements and data analysis suggest that the best fit of the leaching-
rate data is obtained using two exponential functions. This is know as the double-
exponential model: 5
1 2 β β
1 2(1 ) (1 ) t t
C C e C e . (3.2)
C∞1 + C∞2 is the saturated concentration and β1 and β2 are the time constants.
Figure 3.4 shows the leaching amount of anion from PAR-817 resist as a function
of the water contact time. These results were measured via the DLP method at
IMEC. Both the single-exponential model (Eq. (3.1)) and the double-exponential
Figure 3.3 Dynamic model of PAG leaching.
Resist Leaching and Water Uptake 57
model (Eq. (3.2)) were used to fit the measured data points shown in Figs. 3.4(a)
and (b)). The correlation coefficients (R 2 ) show that the double-exponential
model fits the original data better than does the single-exponential model.
The double-exponential model suggests two processes, one fast and one slow,
that could play a role in resist leaching. The fast leaching process occurs
immediately after the water contacts the resist and reaches saturation within a
few seconds, while the slow leaching process lasts much longer, up to 5–20
minutes. The fast process may be a result of PAG that has accumulated near the
resist–air interface during spin-coating and baking. The slow process may be a
result of PAG leaching from within the bulk of the resist. 8 This mechanism
explains why some residual leaching can be observed even after long pre-soaks.
Finite element modeling suggests that PAG initially located at the surface
quickly diffuses into the water. 9 However, the diffusion coefficients of PAG in
the bulk are much smaller than they are within the surface region. These results
are consistent with the experimental observations that leaching is best described
by two time constants (Eq. (3.2)). One corresponds to the leaching of PAGs from
the surface, the other corresponds to the leaching of PAGs from the bulk.
Figure 3.4 Leaching amount of anion from PAR-817 resist as a function of the water contact
time (dots in the figures). The curve in (a) is the fitted results (C∞ = 5.6 × 10 -11
mol/cm 2 , β =
) using the single-exponential model. The curve in (b) is the fitted results (C∞1 = 3.5×10
2 , β1 = 0.15s
-1 ; C∞2 = 3.4×10
2 , β2 = 0.0035s
-1 ) using the double-
exponential model. (Reprinted by permission from Ref. 5.)
58 Chapter 3
In a full-field 193-nm immersion scanner, the exposure head stays in one
field only for a few seconds. Therefore, the fast leaching process is a particularly
important factor in understanding lens contamination. The single-exponential
model and dynamic leaching rate proposed in Eq. (3.1) are sufficient for studying
leaching kinetics relevant to lens contamination. The slow leaching occurs in the
time scale o